Rutting Prediction of Asphalt Mixtures Modified by Polypropylene Fibers via Repeated Creep Testing by Utilising Genetic Programming
Serkan Tapkna*, Abdulkadir evikb, n Uara, Eren Glanc
aCivil Engineering Department, Anadolu University, Eskiehir 26555, Turkey bCivil Engineering Department, University of Gaziantep, Gaziantep 27310, Turkey
cCivil Engineering Department, Gazikent University, Gaziantep 27410, Turkey
Received: May 24, 2012; Revised: September 3, 2012
A novel application of genetic programming (GP) for modelling and presenting closed form solutions to the rutting prediction for polypropylene (PP) modified asphalt mixtures is investigated. Various PP fibers have been utilised for bitumen modification and repeated creep (RC) tests have been carried out. Marshall specimens, fabricated with multifilament 3 mm (M-03) type PP fibers at optimum bitumen content of 5% have been tested under different load values and patterns at 50 C to investigate their rutting potential. It has been shown that the service lives of PP fiber-reinforced Marshall specimens are respectively longer than the control specimens under the same testing conditions (5 to 12 times). Input variables in the developed GP model use the physical properties of Marshall specimens such as PP type, specimen height, unit weight, voids in mineral aggregate, voids filled with asphalt, air voids, rest period and pulse counts. The performance of the accuracy of the proposed GP model is observed to be quite satisfactory. To obtain the main effects plot, detailed parametric studies have been performed. The presented closed form solution will also help further researchers willing to perform studies on the prediction of the rutting potential of asphalt without carrying out destructive tests for similar type of aggregate sources, bitumen, aggregate gradation, modification technique and laboratory conditions.
Keywords: asphalt, polypropylene fibers, rutting potential, genetic programming, modelling, closed form solutions
1. IntroductionIn this study, a genetic programming (GP) model
has been proposed to predict the strain accumulation (rutting potential) developed in the polypropylene (PP) fiber modified Marshall specimens during repeated load creep tests. The proposed study differs from the previous researches in the sense that, no studies have been carried out for the prediction of the RC test results with the aid of GP, closed form solutions and parametric studies carried out on Marshall specimens fabricated in the laboratory environment up to date.
The first part of this study gives short information on creep (basically repeated) testing of asphalt spanning in the last two decades about the actual loading simulation efforts. Then, well known applications of GP techniques in pavement engineering are explored. Next, experimental program presenting the results of the RC tests has been stated in a detailed manner. At this point, a very general overview of GP is presented. Expression tree for the strain accumulation under various RC loading patterns is given in the next section. In order to obtain the main effects plot, a wide range of parametric studies have been performed by using the GP models. The analysis of these results is presented next. Finally, the MATLAB code for the closed form solutions of the prediction of rutting potential is given in Appendix 1.
2. The Idea Behind the Repeated Creep Testing Procedure and Recent LiteratureIn the undertaken RC studies, first of all, the testing
temperature was chosen as 50 C to simulate actual in-situ conditions. An axial stress, , of 500 kPa was applied to the specimens until the specimen enters the tertiary creep region to nearly a failure point to simulate the actual in-place conditions in a realistic manner1-3. Universal testing system (UTM) was utilised in order to log the accumulation mechanisms of the developing strains or in other words rutting potential. Prior to testing, the specimens were put into the chamber of UTM for 24 hours in order to have uniform temperature distribution. To understand the behaviour of the asphalt specimens under different loading patterns, different constant stress values were chosen (namely 100, 207 and 500 kPa). As PP fiber modification was carried out, utilizing lower stress values like 100 and 207 kPa was not feasible, since under such loading the tertiary creep region could not be observed within a reasonable period of time3. Therefore, in order to be able to differentiate between the reference and fiber-reinforced samples, a real destructive loading level of 500 kPa (approximately 73 psi) was chosen as the standard stress value which is a main departure from the published pioneering literature of the rule of thumbs about creep testing3. This value very well represents the actual tire pressure of a loaded truck. The specimen strain
DI:D 10.1590/S1516-14392013005000012Materials Research. 2013; 16(2): 277-292 2013
Tapkn et al.
during the pulsed loading stage of the test were measured in the same axis as the applied stress using two linear variable displacement transducers (LVDTs). The applied force was open loop controlled and rectangular in shape. Load periods were chosen as 500 ms for all of the specimens and the rest periods were 500, 1000, 1500 and 2000 ms, respectively. Four specimens were tested for each loading pattern3.
Matthews and Monismith4 have performed unconfined creep tests at temperatures 25 C, 38 C and 49 C which is a main departure from the published literature up to date in the testing temperature manner. In another study by Mallick et al.5, in order to simulate the average pavement temperature throughout the United States, 60 C of testing temperature was utilised. Ramsamooj and Ramadan6 had carried out creep tests at four stress levels under constant stresses of 150, 400, 650 and 900 kPa. Zhang et al.7 had utilised a material testing system to conduct RC tests. The test temperature was 60 C. Test loading consisted of a 138 kPa (20 psi) confining pressure and an 827 kPa (120 psi) normal pressure. Tashman et al.8 had carried out triaxial confined static creep test in determining the model parameters related to their studies. Chen et al.9 had investigated the mechanical responses and modelling of rutting in flexible pavements. Goh and You10 has revised the RC testing ambient temperature in a different manner than only utilising 40C. Vardanega et al.11 have used a very similar ambient temperature and loading pattern to Tapkn et al. in the studies that they have carried out (namely 50 C and 0.5 (also 1.5) second loading and 1.5 (also 0.4) second unloading) depending on the argument which is also verified by the experience of QDMR (Queensland Department of Main Roads). Chen et al.12 investigated the utilization of recycled brick powder as alternative filler in asphalt mixture. They had carried out static and dynamic creep tests using UTM.
3. Recent Genetic Programming Studies Carried Out in Pavement Engineering ApplicationsSundin and Braban-Ledoux13 have summarized
the findings of up to date research articles concerning the application of artificial intelligence to pavement management and to illustrate the potential of such tools. Hadi and Arfiadi14 have mentioned about the design of rigid pavements according to AUSTRDADS. A genetic algorithm is used to find the optimum design. Chan et al.15 have tried to solve the problem of pavement maintenance management at the network level and genetic algorithms (GAs) have been demonstrated to be better than traditional techniques in terms of solution quality and diversity. Tack and Chou16 have described in their studies, the development of a GA based optimization tool for determining the optimal multiyear pavement repair schedule. Tsai et al.17 have demonstrated the applicability of the GA to solve nonlinear optimization problems encountered in asphalt pavement design. Tsai et al.18, furthermore, inspected the three stage Weibull equation and tree based model to characterize the mix fatigue damage process. In another study by Alavi et al.19, a high precision model was derived
to predict the flow number of dense asphalt mixtures using a novel hybrid method coupling GP and simulated annealing. Gandomi et al.20 also developed a novel hybrid method coupling GP and orthogonal least squares. In another paper by Gandomi and Alavi21, a new approach for behavioural modelling of structural engineering systems is presented using a promising variant of GP, namely multi-gene GP (MGGP). In the second part of their studies, this time, Gandomi and Alavi22 present an endeavour to exploit a robust MGGP method for the analysis of geotechnical and earthquake engineering systems. Finally, Jorge and Ferreira23 present a new maintenance optimisation system, called GENEPAV-HDM4, which was developed to integrate the pavement management system of the municipality of Viseu (Portugal).
4. Experiments Carried OutContinuous aggregate gradation has been used to fit the
gradation limits for wearing course Type 2 set by General Directorate of Turkish Highways24. The aggregate was a calcareous type crushed stone obtained from a local quarry and 50/70 penetration bitumen was obtained from a local refinery were used. Physical properties of the bitumen samples are given in Table 1. The physical properties of coarse and fine aggregates are given in Tables 2 and 3. The apparent specific gravity of filler is 2790 kg.m3. The mixture gradation and gradation limits are given in Table 4.
Table 1. Physical properties of the reference bitumen.
Penetration at 25 C (1/10 mm) 55.4 ASTM D 5-97Penetration index 1.2 -
Ductility at 25 C (cm) >100 ASTM D 113-99Loss on heating (%) 0.057 ASTM D 6-80Specific gravity at 25 C ( kg.m